LMucko/crystallography-open-database huggingface dataset:
Synthesis and structure of anhydrous rare-earth perchlorates M (Cl O4)3 (M = La, Ce-Er, Y): derivatives of the U Cl3 type structure
Wickleder, M.S.; Schaefer, W.; Zeitschrift fuer Anorganische und Allgemeine Chemie 625 (1999) 309–312; doi:

data_1522169
_publ_section_title
;
 Synthesis and structure of anhydrous rare-earth perchlorates M (Cl O4)3
 (M = La, Ce-Er, Y): derivatives of the U Cl3 type structure
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              309
_journal_page_last               312
_journal_volume                  625
_journal_year                    1999
_chemical_formula_sum            'Cl3 Er O12'
_chemical_name_systematic        'Er (Cl O4)3'
_space_group_IT_number           176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   9.197
_cell_length_b                   9.197
_cell_length_c                   5.597
_cell_volume                     409.995
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Wickleder_ZAACAB_1999_859.cif
_cod_data_source_block           Cl3Er1O12
_cod_original_cell_volume        409.9947
_cod_original_formula_sum        'Cl3 Er1 O12'
_cod_database_code               1522169
Superconductivity of some alloys of the systems Nb3 Ga - Nb3 Pt and V3 Ga - V3 Pt
Kopetskii, C.V.; Pavlyuchenko, A.V.; Fizika Metallov i Metallovedenie 43 (1977) 498–502; doi:

data_1522170
_publ_section_title
;
 Superconductivity of some alloys of the systems Nb3 Ga - Nb3 Pt and V3 Ga
 - V3 Pt
;
_journal_name_full               'Fizika Metallov i Metallovedenie'
_journal_page_first              498
_journal_page_last               502
_journal_volume                  43
_journal_year                    1977
_chemical_formula_sum            'Ga0.29 Pt0.71 V3'
_chemical_name_systematic        '(Ga0.29 Pt0.71) V3'
_space_group_IT_number           223
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.814
_cell_length_b                   4.814
_cell_length_c                   4.814
_cell_volume                     111.563
_citation_journal_id_ASTM        FMMTAK
_cod_data_source_file            Kopetskii_FMMTAK_1977_322.cif
_cod_data_source_block           Ga0.29Pt0.71V3
_cod_original_cell_volume        111.5625
_cod_database_code               1522170
Synthesis, structure, and magnetic behavior of La5 Re3 Mn O16: a new perovskite-like material
Wiebe, C.R.; Gourrier, A.; Langet, T.; Britten, J.F.; Greedan, J.E.; Journal of Solid State Chemistry 151 (2000) 31–39; doi:

data_1522171
_publ_section_title
;
 Synthesis, structure, and magnetic behavior of La5 Re3 Mn O16: a new
 perovskite-like material
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              31
_journal_page_last               39
_journal_volume                  151
_journal_year                    2000
_chemical_formula_sum            'La5 Mn O16 Re3'
_chemical_name_systematic        'La5 (Re3 Mn O16)'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1 (1/2*x+1/2*y,1/2*x-1/2*y,-z)'
_symmetry_space_group_name_H-M   'C -1'
_cell_angle_alpha                90.2
_cell_angle_beta                 95.16
_cell_angle_gamma                89.92
_cell_formula_units_Z            2
_cell_length_a                   7.9885
_cell_length_b                   8.0322
_cell_length_c                   10.2413
_cell_volume                     654.468
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Wiebe_JSSCBI_2000_1871.cif
_cod_data_source_block           La5Mn1O16Re3
_cod_original_cell_volume        654.4679
_cod_original_sg_symbol_H-M      'P -1 (a+b,a-b,-c)'
_cod_original_formula_sum        'La5 Mn1 O16 Re3'
_cod_database_code               1522171
Phase diagram and physical properties of Ni-Ru alloys
Kornilov, I.I.; Myasnikova, K.P.; Izvestiya Akademii Nauk SSSR, Otdelinie Tekhnicheskikh Nauk 1964 (1964) 159–165; doi:

data_1522172
_publ_section_title
;
 Phase diagram and physical properties of Ni-Ru alloys
;
_journal_name_full
;
Izvestiya Akademii Nauk SSSR, Otdelinie Tekhnicheskikh Nauk
;
_journal_page_first              159
_journal_page_last               165
_journal_volume                  1964
_journal_year                    1964
_chemical_formula_sum            'Ni0.8 Ru0.2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.583
_cell_length_b                   3.583
_cell_length_c                   3.583
_cell_volume                     45.998
_citation_journal_id_ASTM        IANTA8
_cod_data_source_file            Kornilov_IANTA8_1964_1471.cif
_cod_data_source_block           Ni0.8Ru0.2
_cod_original_cell_volume        45.99815
_cod_database_code               1522172
Pressure-induced structural phase transitions in Ln2-x Ndx Cu O4 for Ln= La (0.6< x<2) and Ln= Pr (x= 0)
Wilhelm, H.; Cros, C.; Reny, E.; Demazeau, G.; Hanfland, M.; Journal of Solid State Chemistry 151 (2000) 231–240; doi:

data_1522173
_publ_section_title
;
 Pressure-induced structural phase transitions in Ln2-x Ndx Cu O4 for Ln=
 La (0.6< x<2) and Ln= Pr (x= 0)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              231
_journal_page_last               240
_journal_volume                  151
_journal_year                    2000
_chemical_formula_sum            'Cu La Nd O4'
_chemical_name_systematic        '(La Nd) Cu O4'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.9746
_cell_length_b                   3.9746
_cell_length_c                   12.3647
_cell_volume                     195.331
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Wilhelm_JSSCBI_2000_1856.cif
_cod_data_source_block           Cu1La1Nd1O4
_cod_original_cell_volume        195.3307
_cod_original_formula_sum        'Cu1 La1 Nd1 O4'
_cod_database_code               1522173
New hydride phases in the systems R-Mg-H (R= Y, La, Ce)
Kost, M.E.; Kuznetsov, N.T.; Shilov, A.L.; Doklady Akademii Nauk SSSR 292 (1987) 632–634; doi:

data_1522174
_publ_section_title
;
 New hydride phases in the systems R-Mg-H (R= Y, La, Ce)
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              632
_journal_page_last               634
_journal_volume                  292
_journal_year                    1987
_chemical_formula_sum            'La Mg2'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.774
_cell_length_b                   8.774
_cell_length_c                   8.774
_cell_volume                     675.450
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Kost_DANKAS_1987_899.cif
_cod_data_source_block           La1Mg2
_cod_original_cell_volume        675.4495
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'La1 Mg2'
_cod_database_code               1522174
Classical antiferromagnetism in the Tb Ni Ga compound
Kotsanidis, P.A.; Yakinthos, J.K.; Journal of Magnetism and Magnetic Materials 81 (1989) 159–162; doi:

data_1522175
_publ_section_title
;
 Classical antiferromagnetism in the Tb Ni Ga compound
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              159
_journal_page_last               162
_journal_volume                  81
_journal_year                    1989
_chemical_formula_sum            'Ga Ni Tb'
_chemical_name_systematic        '(Ga Ni) Tb'
_space_group_IT_number           74
_symmetry_space_group_name_Hall  '-I 2b 2'
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.302
_cell_length_b                   6.88
_cell_length_c                   7.347
_cell_volume                     217.455
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Kotsanidis_JMMMDC_1989_280.cif
_cod_data_source_block           Ga1Ni1Tb1
_cod_original_cell_volume        217.4548
_cod_original_formula_sum        'Ga1 Ni1 Tb1'
_cod_database_code               1522175
Pressure-induced structural phase transitions in Ln2-x Ndx Cu O4 for Ln= La (0.6< x<2) and Ln= Pr (x= 0)
Wilhelm, H.; Cros, C.; Hanfland, M.; Reny, E.; Demazeau, G.; Journal of Solid State Chemistry 151 (2000) 231–240; doi:

data_1522176
_publ_section_title
;
 Pressure-induced structural phase transitions in Ln2-x Ndx Cu O4 for Ln=
 La (0.6< x<2) and Ln= Pr (x= 0)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              231
_journal_page_last               240
_journal_volume                  151
_journal_year                    2000
_chemical_formula_sum            'Cu La Nd O4'
_chemical_name_systematic        '(La Nd) Cu O4'
_space_group_IT_number           64
_symmetry_space_group_name_Hall  '-C 2ac 2'
_symmetry_space_group_name_H-M   'C m c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.2431
_cell_length_b                   12.7848
_cell_length_c                   5.2931
_cell_volume                     354.807
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Wilhelm_JSSCBI_2000_1859.cif
_cod_data_source_block           Cu1La1Nd1O4
_cod_original_formula_sum        'Cu1 La1 Nd1 O4'
_cod_database_code               1522176
The crystal structure of Sc29 Fe6
Kotur, B.Ya.; Bodak, O.I.; Andrusyak, R.I.; Zavodnik, V.E.; Bel'skii, V.K.; Dopovidi Akademii Nauk Ukrains'koi RSR, Seriya B: Geologichni, Khimichni ta Biologichni Nauki 1986 (1986) 29–32; doi:

data_1522177
_publ_section_title
;
 The crystal structure of Sc29 Fe6
;
_journal_name_full
;
Dopovidi Akademii Nauk Ukrains'koi RSR, Seriya B: Geologichni, Khimichni ta 
Biologichni Nauki
;
_journal_page_first              29
_journal_page_last               32
_journal_volume                  1986
_journal_year                    1986
_chemical_formula_sum            'Fe6 Sc29'
_space_group_IT_number           200
_symmetry_space_group_name_Hall  '-P 2 2 3'
_symmetry_space_group_name_H-M   'P m -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.361
_cell_length_b                   14.361
_cell_length_c                   14.361
_cell_volume                     2961.789
_citation_journal_id_ASTM        DANND6
_cod_data_source_file            Kotur_DANND6_1986_53.cif
_cod_data_source_block           Fe6Sc29
_cod_database_code               1522177
Pressure-induced structural phase transitions in Ln2-x Ndx Cu O4 for Ln= La (0.6< x<2) and Ln= Pr (x= 0)
Wilhelm, H.; Cros, C.; Demazeau, G.; Reny, E.; Hanfland, M.; Journal of Solid State Chemistry 151 (2000) 231–240; doi:

data_1522178
_publ_section_title
;
 Pressure-induced structural phase transitions in Ln2-x Ndx Cu O4 for Ln=
 La (0.6< x<2) and Ln= Pr (x= 0)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              231
_journal_page_last               240
_journal_volume                  151
_journal_year                    2000
_chemical_formula_sum            'Cu O4 Pr2'
_chemical_name_systematic        'Pr2 Cu O4'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.9609
_cell_length_b                   3.9609
_cell_length_c                   12.2395
_cell_volume                     192.022
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Wilhelm_JSSCBI_2000_1860.cif
_cod_data_source_block           Cu1O4Pr2
_cod_original_cell_volume        192.0222
_cod_original_formula_sum        'Cu1 O4 Pr2'
_cod_database_code               1522178
New ternary stannides of scandium and cobalt(nickel,copper)
Kotur, B.Ya.; Klyuchka, I.P.; Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy 25 (1989) 597–599; doi:

data_1522179
_publ_section_title
;
 New ternary stannides of scandium and cobalt(nickel,copper)
;
_journal_name_full
'Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy'
_journal_page_first              597
_journal_page_last               599
_journal_volume                  25
_journal_year                    1989
_chemical_formula_sum            'Ni Sc Sn'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.625
_cell_length_b                   4.333
_cell_length_c                   7.536
_cell_volume                     216.329
_citation_journal_id_ASTM        IVNMAW
_cod_data_source_file            Kotur_IVNMAW_1989_1480.cif
_cod_data_source_block           Ni1Sc1Sn1
_cod_original_cell_volume        216.3294
_cod_original_formula_sum        'Ni1 Sc1 Sn1'
_cod_database_code               1522179
New ternary stannides of scandium and cobalt(nickel,copper)
Kotur, B.Ya.; Klyuchka, I.P.; Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy 25 (1989) 597–599; doi:

data_1522180
_publ_section_title
;
 New ternary stannides of scandium and cobalt(nickel,copper)
;
_journal_name_full
'Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy'
_journal_page_first              597
_journal_page_last               599
_journal_volume                  25
_journal_year                    1989
_chemical_formula_sum            'Ni2 Sc Sn'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.228
_cell_length_b                   6.228
_cell_length_c                   6.228
_cell_volume                     241.572
_citation_journal_id_ASTM        IVNMAW
_cod_data_source_file            Kotur_IVNMAW_1989_1481.cif
_cod_data_source_block           Ni2Sc1Sn1
_cod_original_cell_volume        241.5716
_cod_original_formula_sum        'Ni2 Sc1 Sn1'
_cod_database_code               1522180
Pressure-induced structural phase transitions in Ln2-x Ndx Cu O4 for Ln= La (0.6< x<2) and Ln= Pr (x= 0)
Wilhelm, H.; Cros, C.; Reny, E.; Demazeau, G.; Hanfland, M.; Journal of Solid State Chemistry 151 (2000) 231–240; doi:

data_1522181
_publ_section_title
;
 Pressure-induced structural phase transitions in Ln2-x Ndx Cu O4 for Ln=
 La (0.6< x<2) and Ln= Pr (x= 0)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              231
_journal_page_last               240
_journal_volume                  151
_journal_year                    2000
_chemical_formula_sum            'Cu O4 Pr2'
_chemical_name_systematic        'Pr2 Cu O4'
_space_group_IT_number           64
_symmetry_space_group_name_Hall  '-C 2ac 2'
_symmetry_space_group_name_H-M   'C m c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.25
_cell_length_b                   12.748
_cell_length_c                   5.319
_cell_volume                     355.985
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Wilhelm_JSSCBI_2000_1862.cif
_cod_data_source_block           Cu1O4Pr2
_cod_original_cell_volume        355.9847
_cod_original_formula_sum        'Cu1 O4 Pr2'
_cod_database_code               1522181
New ternary stannides of scandium and cobalt(nickel,copper)
Kotur, B.Ya.; Klyuchka, I.P.; Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy 25 (1989) 597–599; doi:

data_1522182
_publ_section_title
;
 New ternary stannides of scandium and cobalt(nickel,copper)
;
_journal_name_full
'Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy'
_journal_page_first              597
_journal_page_last               599
_journal_volume                  25
_journal_year                    1989
_chemical_formula_sum            'Ni4 Sc Sn'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.897
_cell_length_b                   6.897
_cell_length_c                   6.897
_cell_volume                     328.081
_citation_journal_id_ASTM        IVNMAW
_cod_data_source_file            Kotur_IVNMAW_1989_1482.cif
_cod_data_source_block           Ni4Sc1Sn1
_cod_original_cell_volume        328.0807
_cod_original_formula_sum        'Ni4 Sc1 Sn1'
_cod_database_code               1522182
Synthesis, characterization and structure of SAPO-56, a member of the ABC double-six-ring family of materials with stacking sequence AABBCCBB
Wilson, S.T.; Broach, R.W.; Bateman, C.A.; Blackwell, C.S.; McGuire, N.K.; Kirchner, R.M.; Microporous and Mesoporous Materials 28 (1999) 125–137; doi:

data_1522183
_publ_section_title
;
 Synthesis, characterization and structure of SAPO-56, a member of the ABC
 double-six-ring family of materials with stacking sequence AABBCCBB
;
_journal_name_full               'Microporous and Mesoporous Materials'
_journal_page_first              125
_journal_page_last               137
_journal_volume                  28
_journal_year                    1999
_chemical_formula_sum            'Al24 O96 P24'
_chemical_name_systematic        'Al24 (P O4)24'
_space_group_IT_number           163
_symmetry_space_group_name_Hall  '-P 3 2c'
_symmetry_space_group_name_H-M   'P -3 1 c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   13.7571
_cell_length_b                   13.7571
_cell_length_c                   19.93619
_cell_volume                     3267.583
_citation_journal_id_ASTM        MIMMFJ
_cod_data_source_file            Wilson_MIMMFJ_1999_462.cif
_cod_data_source_block           Al24O96P24
_cod_database_code               1522183
The ternary systems Sc-Y-Si and Sc-Lu-Si
Kotur, B.Ya.; Mokra, I.R.; Neorganicheskie Materialy 30 (1994) 783–787; doi:

data_1522184
_publ_section_title
;
 The ternary systems Sc-Y-Si and Sc-Lu-Si
;
_journal_name_full               'Neorganicheskie Materialy'
_journal_page_first              783
_journal_page_last               787
_journal_volume                  30
_journal_year                    1994
_chemical_formula_sum            'Sc0.86 Si1.76 Y0.14'
_chemical_name_systematic        '(Sc0.86 Y0.14) Si1.76'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.7079
_cell_length_b                   3.7079
_cell_length_c                   3.942
_cell_volume                     46.936
_citation_journal_id_ASTM        NMATEI
_cod_data_source_file            Kotur_NMATEI_1994_516.cif
_cod_data_source_block           Sc0.86Si1.76Y0.14
_cod_original_cell_volume        46.9357
_cod_database_code               1522184
Structure and magnetism in Pr3 Ru O7
Wiss, F.; Raju, N.P.; Wills, A.S.; Greedan, J.E.; International Journal of Inorganic Materials 2 (2000) 53–59; doi:

data_1522185
_publ_section_title
;
 Structure and magnetism in Pr3 Ru O7
;
_journal_name_full
'International Journal of Inorganic Materials'
_journal_page_first              53
_journal_page_last               59
_journal_volume                  2
_journal_year                    2000
_chemical_formula_sum            'O7 Pr3 Ru'
_chemical_name_systematic        'Pr3 (Ru O7)'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.974
_cell_length_b                   7.3908
_cell_length_c                   7.5239
_cell_volume                     610.238
_citation_journal_id_ASTM        IJIMCR
_cod_data_source_file            Wiss_IJIMCR_2000_1689.cif
_cod_data_source_block           O7Pr3Ru1
_cod_original_cell_volume        610.2382
_cod_original_formula_sum        'O7 Pr3 Ru1'
_cod_database_code               1522185
Magnetic properties and crystal-structure transfomations of the orderd alloy (Mn Rh)
Kouvel, J.S.; Hartelius, C.C.; Osika, L.M.; Journal of Applied Physics 34 (1963) 1095–1096; doi:

data_1522186
_publ_section_title
;
 Magnetic properties and crystal-structure transfomations of the orderd
 alloy (Mn Rh)
;
_journal_name_full               'Journal of Applied Physics'
_journal_page_first              1095
_journal_page_last               1096
_journal_volume                  34
_journal_year                    1963
_chemical_formula_sum            'Mn Rh'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.044
_cell_length_b                   3.044
_cell_length_c                   3.044
_cell_volume                     28.206
_citation_journal_id_ASTM        JAPIAU
_cod_data_source_file            Kouvel_JAPIAU_1963_1161.cif
_cod_data_source_block           Mn1Rh1
_cod_original_cell_volume        28.20551
_cod_original_formula_sum        'Mn1 Rh1'
_cod_database_code               1522186